Effect of Vegard strains on the extrinsic size effects in ferroelectric nanoparticles


 April Marianna Foster
 1 years ago
 Views:
Transcription
1 PHYSICAL REVIEW B 90, (2014) Effect of Vegard strains on the extrinsic size effects in ferroelectric nanoparticles Anna N. Morozovska, 1,* Iryna S. Golovina, 2,* Sergiy V. Lemishko, 2,3 Alexander A. Andriiko, 3 Sergiy A. Khainakov, 4 and Eugene A. Eliseev 5 1 Institute of Physics, National Academy of Sciences of Ukraine, 46, pr. Nauki, Kyiv, Ukraine 2 Institute of Semiconductor Physics, National Academy of Sciences of Ukraine, 41, pr. Nauki, Kyiv, Ukraine 3 National Technical University of Ukraine, Kyiv Polytechnic Institute, Kyiv, Ukraine 4 Department of Organic and Inorganic Chemistry, University of Oviedo, Oviedo, Spain 5 Institute of Problems for Material Sciences, National Academy of Sciences of Ukraine, 3, Krjijanovskogo, Kyiv, Ukraine (Received 7 October 2014; revised manuscript received 14 November 2014; published 5 December 2014) By changing the size and the shape of ferroelectric nanoparticles, one can govern their polar properties, including their improvement in comparison with the bulk material. The shift of the ferroelectric transition temperature can reach hundreds of degrees Kelvin. A phenomenological description of these effects was proposed in the framework of LandauGinsburgDevonshire (LGD) theory using the concepts of surface tension and surface bond contraction. However, this description contains a series of poorly defined parameters, and the physical nature is ambiguous. It appears that the size and shape dependences of the phase transition temperature, along with all polar properties, are defined by the nature of the size effect. Existing LGDtype models do not take into account that defect concentration strongly increases near the particle surface. In order to develop an adequate phenomenological description of size effects in ferroelectric nanoparticles, one should consider Vegard strains (local lattice deformations) originating from defect accumulation near the surface. In this paper, we propose a theoretical model that takes into account Vegard strains and performs a detailed quantitative comparison of the theoretical results with experimental ones for quasispherical KTa 1x Nb x O 3 nanoparticles (average radius 25 nm), which reveal the essential (about 100 K) increase of the transition temperature in spherical nanoparticles in comparison with bulk crystals. From the comparison between the theory and experiment, we established the leading contribution of Vegard strains to the extrinsic size effects in ferroelectric nanoparticles. We determined the dependence of Vegard strains on the content of Nb and reconstructed the Curie temperature dependence on the content of Nb using this dependence. The dependence of the Curie temperature on the Nb content becomes a nonmonotonic one for the small (<20 nm) elongated KTa 1x Nb x O 3 nanoparticles. We established that the accumulation of intrinsic and extrinsic defects near the surface can play a key role in the physical origin of extrinsic size effects in ferroelectric nanoparticles and govern its main features. DOI: /PhysRevB I. INTRODUCTION The study of unique physical properties of ferroelectric nanoparticles attracts the attention of researchers. Yadlovker and Berger [1 3] present unexpected experimental results that reveal the enhancement of polar properties of cylindrical nanoparticles of Rochelle salt. The authors of Refs. [4 6] successfully managed the temperature of the ferroelectric phase transition and the magnitude and position of the maximum of the dielectric constant for nanopowders and nanoceramics of barium titanate and lead titanate. The studies of KTaO 3 nanopowders [7 10] and nanograined ferroelectrics of KNbO 3 and KTa 1x Nb x O 3 [11 13] revealed new polar and magnetic phases and the shift of phase transition temperature in comparison with bulk crystals. Theoretical consideration of manifold size effects allows one to establish the physical origin of the transition temperature shift and phase diagram changes appearing under the decrease of nanoparticle sizes. In particular, using the continual phenomenological approach, Perriat et al. [14], Huang et al. [15,16], Morozovska et al. [17,18,20], Eliseev et al. [21], and Ma [22] have shown that the changes of the * Corresponding author: or PACS number(s): Ek, bn transition temperatures and the enhancement or weakening of polar properties are conditioned by different extrinsic and intrinsic size effects in nanoparticles. The partition is tentative and specified by the size effect manifestation. Size effect classification in ferroelectric nanoparticles is given in the first column of Table I. As a rule, the term extrinsic size effects implies that its consequences depend on the size and the shape of the particle but not on its internal state (e.g., not the gradients of physical properties inside the nanoparticle). The contribution of the extrinsic size effecst leads to the shift of the transition Curie temperature from the paraelectric to ferroelectric phase that is proportional to either 1/R [14,17 21]or1/R 2 [15], depending on the model, where R is the curvature radius of the nanoparticles surface (e.g., it is the radius of the spherical particle). For instance, if one considers intrinsic surface stress (see, e.g., Ref. [23]) under the curved surface of solid bodies, it leads to isotropic compression of the particles, resulting in the shift of the transition temperature proportional to Qμ/R, where μ is the coefficient of the surface stress (similar to the surface tension coefficient determining the surface energy in liquids). The form of the effective electrostriction constant Q essentially depends on the shape of the particle, having different signs for the cylinders and spheres of perovskite ferroelectrics [17 21]. In the surface bond contraction model [15], the shift of the Curie temperature is proportional to the ratio χ/r 2, and /2014/90(21)/214103(10) American Physical Society
2 ANNA N. MOROZOVSKA et al. PHYSICAL REVIEW B 90, (2014) TABLE I. Size effects of Curie temperature in ferroelectric nanoparticles. Contribution to size effect (and its origin) Surface stress (from the surface tension) Surface bond contraction (from the surface curvature) Vegard strains/stresses (from defect accumulation) Depolarization, correlation, and spontaneous flexoelectric effects (from electric field and polarization gradients) Size dependence of Curie temperature shift and dependence on the particle radius R Size effect type Ref. Spherical particle of radius R Ellipsoid or wire of radius R with polarization directed along the longer axes L R 2μ(2Q 12+Q 11 ) α T R 4μQ 12 α T R Extrinsic ( 1/R) [17,18] μ is a surface stress (tension) coefficient that is positive, Q ij are electrostriction coefficients, and α T is the temperature coefficient of dielectric stiffness 4Y δa (na) 2 α T a R 2 2Y δa (na) 2 α T Extrinsic ( 1/R 2 ) [15,16] a R 2 Y is the Young modulus, δa is the contraction of a lattice constant a, and n is the number of contracted layers; factor χ = 4Y δa α T a (na)2 2η(Q 11 +2Q 12 ) R0 2 4ηQ 12 R α T (s 11 +2s 12 ) R α T (s 11 +s 12 ) η is the Vegard strain, R 0 is the defect layer thickness, and s ij are elastic compliances (g/α T ) (g/n d )+(λ+ g/n d )(R/3) λ>0 1 n d = (ε b +2ε e)ε 0 is a depolarization factor ( 2 α T g R 2 Extrinsic ( 1/R 2 ) This work Rλ+R 2 /4 ), λ > 0, ( ) 2 α T g 2λ R 2Rλ, λ < 0. 2 The shift from the depolarization field is negligibly small, and absent in the limit of a wire when L/R λ is the extrapolation length, g is the polarization gradient term, n d is a depolarization factor, ε b is the background permittivity of ferroelectrics [28], and ε e is the permittivity of external media Intrinsic (R dependence is complex) [17,18,27] the value of the factor χ is determined by the surface bond contraction to the lattice parameter ratio δa/a [Table I]. The influence of extrinsic size effects is essential for the particles with a curvature radius (or size) smaller than nm. The known intrinsic size effects of ferroelectric nanoparticles are determined mainly by the longrange gradient of the depolarizing electric field inside the particle and the shortrange (or chemical ) polarization gradient near the surface [24]. They lead to the more complicated dependence of the transition temperature on the shape and size of the particles, primarily due to a nontrivial dependence of the electrical depolarization fields and flexoelectric strains on particle shape, the orientation of the ferroelectric polarization, and the conditions of its screening near the particle surface [17 21]. As a rule, the influence of intrinsic size effects is essential for the particles with sizes less than 10 nm; the internal scale of polarization is determined by the correlation length, which is typically less than 0.5 nm in spherical particles due to the depolarization effect; and the deviation from the bulk polarization is governed by the socalled extrapolation length λ that is about nm [25,26]. Therefore, the analysis of the experimentally observed transition temperature dependence on the particles sizes allows one to establish the nature of size effects in the studied system and to determine corresponding phenomenological parameters like μ, χ, orλ from the fitting of experimental data with the adequate theoretical model. Despite this, it remains to be realized for the majority of nanostructured systems. Probably, the difficulties are mostly due to existing phenomenological considerations of ferroelectric particles not being adequate for real nanoparticles with strongly strained nearsurface layers, where the strains or stresses are caused by the accumulation of defects (impurities and vacancies) in the region. Indeed, it is well established that the defects concentration noticeably increases near the particle surface, allowing for the essential lowering of their formation energies [27 29]. The abrupt, spontaneous polarization near the surface of ferroelectrics causes the strong accumulation of ions and charged vacancies in the spatial regions to screen the bond surface charges [30 33]. In turn, vacancies and ion accumulations near the surfaces of solids produce surface stresses [34] that substantially alter thermodynamic equilibrium [35], leading to the changes of phase diagrams and transition temperatures. In order to develop an adequate thermodynamic description of size effects in ferroelectric nanoparticles, one has to determine the microscopic nature of phenomenological parameters and relate them to the lattice deformation near the particle surface due to the defect accumulation. The analysis of our experimental results has shown that the concept of compositionally induced expansion [34] (or chemical pressure [36]) originated from the Vegard strains [37,38] is consistent with our model. According to this concept, the inclusion of a defect
3 EFFECT OF VEGARD STRAINS ON THE EXTRINSIC... PHYSICAL REVIEW B 90, (2014) FIG. 1. (a) Sequence of phase and structural transformations in KTa 1x Nb x O 3. (b) Intrinsic defects in KTa(Nb)O 3 lattice. (c) and (d) Local lattice deformations caused by intrinsic [oxygen and potassium vacancies, V (O) and V (K)] and extrinsic (Fe 3+ or Mn 2+ ions) defects. (impurity ion or vacancy) leads to the local deformation of the crystal lattice, and the action of many defects causes a strain proportional to their concentration. In this case, the proportionality coefficient is determined either from ab initio calculations [38] or from experiments [39,40]. It should be noted that the influence of the Vegard strain, coming from the diffusion and the accumulation of defects near the interfaces of ferroelectric thin films, results in the pronounced change of their polar properties [41,42]. Therefore, it is natural to expect that one could not neglect Vegard strains when describing polar properties of ferroelectric nanoparticles. Also, a steric effect [43,44] takes place for the strong accumulation ( crowding ) of defects. Thus, we performed the modeling of the transition temperatures for ferroelectric nanoparticles taking into account the Vegard strains. Theoretical results are analyzed and compared with the experiment for KTa 1x Nb x O 3 nanoparticles. II. THEORETICAL MODEL A. Model background for the KTaO 3 KNbO 3 system It was experimentally established that extrinsic and intrinsic defects play a crucial role in the emerging of polar properties in KTa 1x Nb x O 3 nanocrystals [8 10,13]. Thus, due to the presence of the dipole centers associated with Fe 3+ ions (the centers of axial and rhombic symmetries), ferroelectric phase transition occurs in nanocrystalline KTaO 3 at 29 K [7,8], while the bulk material is a quantum paraelectric [45]. These centers include oxygen vacancies in their structure and are formed mainly near the surface of the particles, as the concentration of oxygen vacancies has a sharp maximum in the surface layer. Note the main features of polar and structural phase transitions in the considered system. Bulk KTaO 3 is a quantum paraelectric having a cubic structure down to 0 K [45]. At the same time, KNbO 3 and solid solutions of KTa 1x Nb x O 3 (x>0.2) undergo three successive phase transitions, namely, from the cubic paraelectric to tetragonal ferroelectric phase at Curie temperature (T C ) and then two structural transitions, with the polarization vector Р, switching between different crystallographic directions [Fig. 1(a)]. Also, as shown in Ref. [46], T C shifts almost linearly under the changes of the Nb content x in the KTa 1x Nb x O 3 solid solution. Below we consider the dependence of the Curie temperature on the composition under the decreasing size of the crystals for two particle shapes. In the solid solutions considered, the most prevalent intrinsic defects are vacancies of oxygen and potassium [Fig. 1(b)]. Iron and manganese ions are mostly registered among the extrinsic defects [Figs. 1(c) and 1(d)], which are incorporated into the lattice during the synthesis as unavoidable impurities [9,13]. Figure 1(b) gives an idea of the atomic arrangement and intrinsic defects (oxygen and potassium vacancies) in the KTa(Nb)O 3 lattice. Figure 1(c) demonstrates different possibilities of lattice strain appearance in the presence of an impurity Fe 3+ ion and/or potassium vacancy. In the first case, the Fe 3+ ion occupies a site of the potassium ion K +, and an oxygen ion invades as the charge compensator in the nearest intersite, which leads to strong local stretching of the lattice. The local lattice contraction occurs under the potassium vacancy formation. Corresponding atomic displacements are indicated by arrows. Figure 1(d) demonstrates the different possibilities of lattice strain in the presence of an impurity Mn 2+ ion and/or oxygen vacancy. In the first case, the Mn 2+ ion occupies the site of the Ta 5+ /Nb 5+ ion, and an oxygen vacancy is formed as a charge compensator in the immediate environment. The result is a local extension of the lattice around the impurity ion and its local contraction around oxygen vacancy. Corresponding atomic displacements are indicated by arrows. It is known that the concentration of defects inside the crystal is inhomogeneous and strongly increases from the bulk to the surface of the particle [34,35]. Since the nearsurface
4 ANNA N. MOROZOVSKA et al. PHYSICAL REVIEW B 90, (2014) layer is enriched with defects, here the crystal lattice becomes either spongy or denser depending on the type of defect [Figs. 1(b) 1(d)], meaning that the lattice parameter is also locally changed. With the presence of different types of defects, resulting in either expansion or compression of the lattice, the surface of the particle may have a complicated relief structure. However, the ensemble of weakly interacting or noninteracting particles most probably can be considered as an effective ensemble of ellipsoids with different aspect ratios of the semiaxes R and L. In our calculations, we change the curvature of the surface 1/R and calculate the Curie temperature for two limiting forms of the particle, namely the sphere and very prolate ellipsoid. Thus, R is either the sphere radius or the smaller semiaxis of the ellipsoid hereinafter. B. Basic equations 1. Core and shell model for Vegard pressure calculations Possible lattice deformations caused by intrinsic [vacancies V (O) and V (K)] and extrinsic (Fe 3+ or Mn 2+ ions) defects are shown in Figs. 1(b) 1(d). Following Huang et al. [15] and using the concept of compositionally induced expansion or contraction introduced by Sheldon and Shenoy [34], the defect accumulation under a curved surface produces effective stresses of the inner part of the particle. The screening of the depolarization field at the surface and outside of the particle leads to the exponential decrease of charged defect concentration when moving away from the surface [34]. In addition, the characteristic thickness of the layer enriched by defects is determined by the screening length, and their maximal concentration is limited by a steric effect [41,42]. Based on the abovementioned results, we perform an elementary speculation leading to the semipostulated expression for the hydrostatic pressure acting on the inner part of an ellipsoidal particle with semiaxes R and L(R L) [Fig. 2]. In accordance with the Vegard law [37], local changes in the concentration of defects lead to the appearance of additional sources for elastic strains δη ij = W ij d δn d, where Wij d are the Vegard stress tensor components for defects of the type d ; δn d ( r) = N d ( r) N de is the difference between the instant concentration of defects N d (r) in the point r and their equilibrium (average) concentration N de. Hereinafter, the Vegard tensor is diagonal, i.e., W ij d = Wδ ij (δ ij is the Kronecker delta symbol). For perovskites ABO 3, the absolute values of W related to vacancies can be estimated as W ( ) Å 3 [38], and so the corresponding strains δu ij (r) can reach percentages for a high variation of defect concentration δn d m 3. Assuming that most defects are located in the ultrathin layer under the particle surface and their concentration decreases exponentially towards the particle bulk [34], we can approximately consider the particle consisting of an ultrathin shell of thickness R 0 R highly enriched by defects and the remaining core of radius R R 0 R without them, i.e., δn d = 0 in the core and δn d = N d in the shell. Depending on the Vegard stress sign, the mechanism leads to the tangential compressive or tensile strain δη 11 = δη 22 = WδN d, which exists in the shell of thickness R 0. For the sake of brevity, the strain is further denoted as η, i.e., η WδN d. Then, using eqs. (1) and (3) FIG. 2. (Color online) Schematics of an ellipsoidal particle with semiaxes R and L covered by the shell of thickness R 0, with accumulated defects. Separation between the screening charge and the spontaneous and abrupt polarization at the coreshell interface is R S. Ferroelectric polarization is directed along the longest ellipsoid axes. from Huang et al. [15] and exactly following their derivation in the paper, the deformation η leads to the changes of the spherical particle radius for the value δr = ηr 0 and thus to the appearance or tangential and normal stresses σ tt = Y δr R and σ rr = Y δr R 0, correspondingly, where Y is the Young modulus. To adjust our results with notations used in Ref. [15], note R R that R = Na, δr = nδa, and so n/n R 0 /R. Finally, using Y = 1/(s 11 + s 12 ) and for cubic symmetry, while it should be substituted by the factor for a wire Y 1/(s s 12 ) [17], the hydrostatic pressure acting on the inner part of the ellipsoidal particle with semiaxes R and L acquires the form σ rr (R,x) = { η(x) R0 2(x) s 11 (x)+s 12 (x) η(x) s 11 (x)+2s 12 (x), R L (prolate ellipsoid), R 2 R0 2(x), R L (sphere). R 2 Here, subscript rr denotes that the pressure is radial, and R is the particle radius. s ij (x) is the elastic compliance modulus of the material, and the characteristic size R 0 (x) is the particle surface layer thickness, where accumulated defects create elementary volume changes. Parameter η (x) is a compositional Vegard strain [36 38] that is usually dependent on the Nb content x in KTa 1x Nb x O 3 due to the strong dependence of the elementary volume changes on defect and surrounding atoms type [38]. Immediately, the Vegard strain x dependence can lead to the analogous dependence of the shell thickness R 0 (x). Moreover, the following correlation should exist: the higher the Vegard strain, the thicker the shell, because more numbers of layers are required for the full relaxation of the surface strain. Note that the stress σ rr in Eq. (1) is radius (R) and content (x) dependent; and its x dependence can be determined from our experimental data. With increasing R, the stress decreases proportionally to the ratio (R 2 0 /R2 ). (1)
5 EFFECT OF VEGARD STRAINS ON THE EXTRINSIC... PHYSICAL REVIEW B 90, (2014) 2. Model for depolarization field calculations in ferroelectric nanoparticles covered with a paraelectric shell In accordance with the Poisson equation divd = ρ free,an internal electric field is inevitably present in a nanoparticle with inhomogeneous polarization P that creates nonzero divergence inside the particle, divp 0, as well as when the polarization normal component is abrupt at the particle surface [17 20], and the field is depolarizing. The field is exactly zero only for the case of the ferroelectric nanowire with polarization directed along its axis [17]; it can be regarded negligibly small for ellipsoidal particles with semiaxes R and L and polarization directed along the long axes L, if the aspect ratio R/L is very high (more than 10 3 ). Since we postulated the shell layer enriched by defects, the strong polarization gradient is very likely here. First, let us estimate the maximal depolarization field created by an ellipsoidal singledomain ferroelectric nanoparticle core with uniform polarization P = (0,0,P 3 ) directed along its longer axes L, relative dielectric permittivity ε33 core, and without free carriers. The core is covered by a nonferroelectric paraelectric shell with relative dielectric permittivity ε33 shell, and in addition, the strong inequality ε33 shell ε33 core is likely when the shell is regarded to be in a paraelectric phase close to the ferroelectric transition. The screening charge is located either immediately outside the shell or near its outer surface, so the effective separation between the screening charge and the spontaneous and abrupt polarization at the coreshell interface is R S and R S R 0. Using the inequalities R 0 R<L, the local situation is similar to the planar ferroelectric capacitor of thickness L with a dielectric gap of thickness R S and a depolarization field E3 d = R S P 3 ε 0(R S ε33 core+lεshell 33 ) [28], where ε 0 is a universal dielectric constant. It is shown that the electrostatic problem in Fig. 2 can be solved exactly for a spherical particle, i.e., E3 d = (R 3 (R R S ) 3 )P 3 where R = L. Using ε 0 ((R R S ) 3 (ε33 shell ε33 core)+r3 (2ε33 shell +ε33 core)) the expression and interpolation for ellipsoid depolarization field factors [47] proposed in Ref. [17], n D (a) a 2 /(1 + a 2 ), where a = R/L, we obtain the upper estimation for the depolarization field of the ferroelectric ellipsoid covered with the paraelectric shell R S RP 3, R L (very prolate ellipsoid), E3 d ε 0 ε33 shell L 2 2R S P 3, R L (sphere). (2) 3ε 0 ε33 shell R In reality, expression (2) gives the upper estimation of the depolarization field. In particular, if the shell is semiconducting, the value R S acquires the sense of the ThomasFermi screening radius that can be much smaller than the lattice constant [48]. Also, the difference of core and shell averaged polarizations should be included in Eq. (2), i.e., one can substitute P 3 (P 3 P3 shell ). 3. LandauGinsburgDevonshire phenomenological description Since the actual particle sizes for which we have experimental data are higher than 10 nm [Fig. 3(e)], in the following, we can ignore intrinsic size effects that originated from the polarization gradient, so the LandauGinsburg Devonshire (LGD)potential functional for the solid solution of paraelectric and ferroelectric acquires the relatively simple form [17 21]]: = α bulk (T,x) P β(x)p γ (x)p 3 6 P E3 d 3 2 Q ij 33 σ ij P s ij klσ ij σ kl. (3) Here, x is the content of Nb in KTa 1x Nb x O 3. P 3 stands for the uniform polarization, E d 3 is depolarization field, and Q ij kl are electrostriction tensor coefficients. As one can see from Eq. (3), the coefficient α bulk (T,x) becomes renormalized by the stress given by Eq. (1) via the electrostriction effect [17 21], namely, α(t,r,x) = α bulk (T,x) Q ij 33 (x) σ ij (R,x). The coefficient α(t,r,x) depends on temperature T, particle size R, content x, polarization orientation, and other material parameters. For ellipsoidal particles with semiaxes R and L, with polarization uniformly aligned along the longer ellipsoid axis L, the coefficient α(t,r,x) was calculated as ( ) ( xα Tf T T b Tq C + (1 x)αtq 2 coth ( T q ) ) 2T T0 + R S R α = ( ) ( xα Tf T T b Tq C + (1 x)αtq 2 coth ( T q ) ) 2T T0 + 2R S 3ε 0 ε shell R0 2 s 11 (x)+s 12 (x) ε 0 ε shell 33 L 2 + 4η(x)Q 12(x) R 2, R L, + 2η(x)(Q 11(x)+2Q 12 (x)) R R s 11 (x)+2s 12 (x) R 2, R L. Hereinafter, subscripts q and f denote the values related to proper ferroelectrics and quantum paraelectrics, respectively. Note that the KTa 1x Nb x O 3 parent phase has cubic m3m symmetry. Here, TC b is the ferroelectric Curie temperature of the bulk material. In Eq. (4), we used the Barretttype formula for the coefficient α q (T,R) = α Tq ((T q /2) coth(t q /2T ) T 0 ), which is valid for quantum paraelectrics [49] in a wide temperature interval, including low quantum temperatures. T 0 and T q are the extrapolated virtual Curie temperature and characteristic quantum oscillations temperature, respectively. At temperatures T T q /2, the Barrett formulae transform into the classical limit, α q (T,R) α Tq (T T 0 ). Electrostriction tensor coefficients Q ij content x dependence can be regarded as linear Q ij (x) = xq f ij + (1 x) Qq ij. Linear dependences can also be used for elastic compliances s ij (x) = xs f ij + (1 x) sq ij, Vegard strain η (x) = xη f + (1 x) η q, and shell thickness R 0 (x) = xr f + (1 x) R q. The Curie temperature T C (x,r) of the solid solution can be determined from the condition α(t C,R,x) = 0 that in the classical limit, T C T q /2, Rgives evident analytical expressions T C (R,x) = xα Tf TC b+(1 x)α TqT 0 R S R/(ε 0 ε33 shell L 2 ) xα Tf +(1 x)α Tq 4ηQ 12(R 2 0 /R2 ) (s 11 +s 12 )(xα Tf +(1 x)α Tq ), R L, xα Tf T b C +(1 x)α TqT 0 2R S /(3ε 0 ε shell 33 R) xα Tf +(1 x)α Tq 2η(Q 11+2Q 12 )(R 2 0 /R2 ) (s 11 +2s 12 )(xα Tf +(1 x)α Tq ), R L. (5) (4)
6 ANNA N. MOROZOVSKA et al. PHYSICAL REVIEW B 90, (2014) N (arb. units) FIG. 3. (Color online) (a) Curie and ferroelectric transition temperature vs Nb content x in bulk KTa 1x Nb x O 3. Symbols are experimental data from Ref.[46], and solid curves are the theoretical fitting based on Eqs. (1)(5). Abbreviations PE and FE stand for paraelectric and ferroelectric phases. Parameters of the bulk KTaO 3 and KNbO 3 are listed in Table II. (b) Curie temperature vs Nb content x in assemblies of KTa 1x Nb x O 3 nanoparticles. Different symbols (diamonds and bars) are experimental data, solid and dotted curves are theoretical fittings for nanoparticles with radii of 25, 15, and 35 nm, respectively. Fitting parameters are listed in Table III. (c) and (d) TEM images that show the quasispherical and ellipsoidal KTa 1x Nb x O 3 nanoparticles. (e) The size distribution of nanoparticles. Solid red curve is the histogram fitting by polynomialgaussian fit. For the case of the secondorder phase transitions, T C (x,r) is the transition temperature from the ferroelectric to paraelectric phase. For the firstorder phase transitions, the condition α(t C,R,x) = 0 still gives the Curie temperature, but the ferroelectricparaelectric transition temperature T FE (x,r) should be found as a solution of the transcendental equation α(t FE,R,x) = 3β(x) 2 /(16γ (x)). The spontaneous polarization at E = 0isP0 2 = ( β 2 4αγ β)/2γ. As one can see from Eq. (5), the sizedependent shift of the Curie temperature is induced by the joint action of the depolarization field and Vegard strain, and the latter is reflected by the product η(r 0 /R) 2. For the case of the negligible depolarization contribution (e.g., at ε33 shell ), the radius dependence of the Curie temperature shift is governed by the ratio (R 0 /R) 2. Equation (5) shows that the increase of the Curie temperature in comparison with a bulk material can appear under the condition η (x)(q 11 (x) + 2Q 12 (x)) < 0 for spherical particles, or η (x) Q 12 (x) < 0 for ellipsoidal particles with high aspect ratio L/R 1. III. Nb CONTENT AND SIZE DEPENDENCE OF THE NANOPARTICLE TRANSITION TEMPERATURE To fit the experimental dependence of the Curie temperature T C (x) [squares in Fig. 3(a)] and ferroelectric transition temperature T FE (x) [triangles in Fig. 3(a)] on the content x of Nb, we use the interpolate function for T 0 (x) = T 0 (1 + 25(1 x) 0.7 ). Our fitting, based on Eqs. (1) (5), is shown by solid curves for T FE (x) and dotted curves for T C (x). Corresponding parameters of the bulk KTaO 3 and KNbO 3 are listed in Table II. Table II gives us the parameters of the bulk materials, but the composition dependences of the Vegard strain coefficient and shell thickness, which determine the strength of the size effects in nanoparticles in accordance with, e.g., Eq. (4), remain unknown. To obtain the dependences, we performed the comparison with our experiment. The KTa 1x Nb x O 3 nanoparticle fabrication process is described in detail in Refs. [8,11,12]. Examples of transmission electron microscopy (TEM) images, which show the nanoparticles of quasispherical and ellipsoidal shape, can be seen in Figs. 3(c) and 3(d). Most of the fabricated nanoparticles have a quasispherical shape; their radii are distributed around the most probable size of nm [see histogram in Fig. 3(e)]. The full width at halfmaximum (FWHM) of the particle size distribution is about 20 nm. Although there were sizable amounts of large nanoparticles, they contributed almost nothing to the studied size effects, acting as a background and slightly elongating the error bars of the Curie temperature to lower temperatures. Experimentally,
7 EFFECT OF VEGARD STRAINS ON THE EXTRINSIC... PHYSICAL REVIEW B 90, (2014) TABLE II. Parameters of the bulk KTaO 3 and KNbO 3 extracted from Refs. [10,46,50,51]. Physical quantity Quantum paraelectric KTaO 3 Ferroelectric KNbO 3 Coefficient α T α Tq = m/(fk) α Tf = m/(fk) Characteristic temperatures T q = 55 K, T 0 = 15 K T C = 633 K, T FE = 698 K Electrostriction coefficients Q 11 = 0.11 m 4 /C 2, Q 11 = 0.13 m 4 /C 2, Q 12 = m 4 /C 2 Q 12 = m 4 /C 2 Elastic compliances s 11 = Pa 1 s 11 = Pa 1 s 12 = Pa 1 s 12 = Pa 1 the Curie temperature was determined from Raman scattering measurements using a Jobin Yvon/Horiba T64000 triple Raman spectrometer. The temperature dependences of intensity, width, and frequency of relevant modes of the Raman spectra were thoroughly analyzed. The experimental technique was described in detail in Refs. [11,12]. Comparison of the calculated Curie temperature with experimental results for KTa 1x Nb x O 3 nanoparticles is shown in Fig. 3(b). We attributed the diamonds in the figure to experimental data for nanoparticles with the most probable radius of 25 nm. Error bars show the Curie temperature scattering that originated from the particle radii deviation from 25 nm or about ±10 nm that corresponds to the radii from 15 to 35 nm. Solid and dotted curves show the corresponding theoretical fitting for the 25, 15, and 35 nm radii. Note the pronounced increase of the Curie temperature for KTa 1x Nb x O 3 nanoparticles in comparison with a bulk solid solution for x>0.8, leading to a strong enhancement of the ferroelectric properties. Since Q 12 (x) < 0 and Q 11 (x) + 2Q 12 (x) > 0 for all x, the negative Vegard strain η (x) increases the Curie temperature for spherical nanoparticles, and positive strains η (x) increase the temperature for the prolate ellipsoids accordingly per Eq. (5). Note that the depolarization field contribution, proportional to R S /(ε 0 ε33 shell α Tf R), decreases the Curie temperature by hundreds of degrees Kelvin for a spherical nanoparticle with shell permittivity ε33 shell less than 10 3 and the thickness ratio R S /R more than 10 2, but our experiment reveals a noticeable increase of the nanoparticles Curie temperature ( T C ) in comparison with a bulk one (Table III). Moreover, the depolarization field contribution can strongly dominate the Vegard one. Thus, in order to explain the experimental enhancement of T C, we should assume that the depolarization field contribution leads to a Curie temperature decrease much smaller than dozens of degrees Kelvin. This is readily possible for a semiconducting shell with ε33 shell 10 3 and R S /R < Contentdependent parameters determined from the fitting to experiment are listed in Table III. We found out that the best fitting of the Curie temperature for the quasispherical particles of radius (25 ± 10 nm) corresponds to the negative Vegard strain η (x) = 0.01x 0.03 (1 x) and shell thickness R 0 (x) = (2.4x (1 x)) nm. The latter values are quite reasonable and correspond to the 6 to 10unitcellthick shell. As anticipated, effective sphere fractions in the composite appeared rather high, g (x) = 0.95x (1 x), but some small amount of prolate ellipsoidal particles (from 5% to 10%, depending on the content x) exists due to the presence of elongated particles with high aspect ratio L/R 1. Here, an important remark should be made. We failed to fit the experimental data using both effective surface tension and intrinsic size effect models [17,18] for the realistic values of the surface stress coefficient; such a fitting required very high negative values of the coefficient (about (10 20) N/m), which is in contradiction to the surface equilibrium and realistic range of the coefficient +(1 2) N/m in different perovskites and other oxides [22]. Inclusion of the intrinsic size effect (polarization gradient along with induced depolarization field) leads to the correct trend that agrees with the experiment, namely, to the Curie temperature increase with radius decrease, only at negative extrapolation lengths, and the increase becomes noticeable at a particle radius of less than 5 nm. Since there is no solid background for the existence of the negative extrapolation length and the minimal particle radius represented in the histogram is TABLE III. Parameters of the nanosized KTa 1x Nb x O 3 a. Experimental data for Curie temperature in KTa 1x Nb x O 3 Contentdependent parameters determined from the fitting to experiment shown in Fig. 3(b) Content x Curie temperature Sphere fraction Shell thickness Vegard coefficient T C = T C ± T g(x) = xg f + (1 x)g q R 0 (x) = xr f + (1 x)r q η(x) = xη f + (1 x)η q g f = 0.95, g q = 0.9 R f = 4.2 nm, R q = 2.4nm η f = 3%, η q = 1% x = 0.3 T C = (243 ± 30) K nm 1.6% bulk T C = 238 K x = 0.5 T C = (359 ± 40) K nm 2% bulk T C = 351 K x = 1 T C = (748 ± 50) K nm 3% bulk T C = 633 K a To switch off the depolarization contribution, the shell permittivity ε shell 33 was chosen more than 10 4 and R S less than 0.5 nm
8 ANNA N. MOROZOVSKA et al. PHYSICAL REVIEW B 90, (2014) 5 nm [Fig. 3(e)], inclusion of the intrinsic size effect does not help us describe the experiment. In contrast, the model based on the Vegard strain appeared in quantitative agreement with the experimental results for realistic values of all fitting parameters. The surface bond contraction model [15] gives the same radius dependence of the Curie temperature shift as that of the Vegard strainbased model, but it does not allow quantitative fitting of the experimental data dependence on Nb content x, since only the Young modulus Y is x dependent in the factor χ = 4Y δa α T a (na)2 included in the model (see Table I). Substitution of the known dependence Y (x) does not lead to a reasonable fitting. Other factors, such as the surface bond contraction and the lattice parameter, are almost content independent. The surface bond contraction model is probably adequate for the nanoparticles without surface defects. Since we extract the dependence of the Vegard strain and shell thickness on Nb content x from experimental data in an unambiguous way, we can reliably enough reconstruct the impact of size effects on the nanosized KTa 1x Nb x O 3 using these dependences and vary the particle radius and the spheretoellipsoid ratio in the particle assembly, because these factors can be controlled in realistic experiments. Such a procedure allows the opportunity to predict the Vegard strain impact on the extrinsic size effects in nanoparticles. Thus, let us consider a KTa 1x Nb x O 3 nanocomposite, where particle sizes are distributed around the average value, and the particle shape varies, namely, there are some fraction of ellipsoidal and spherical particles in the material, but electric and elastic interaction between the particles can be regarded as small due to the screening effects and surface stresses in the interfacial regions. Using Eqs. (1) (5) and the parameters listed in Tables II and III, we study content and radius dependences of the extrinsic size effects in the composites with the fraction of spheres varying from 100% to 0%. Reconstructed dependences of the Curie temperature on Nb content x and particle radius R are depicted in Figs. 4 and 5. Curie temperature increases with the increase of Nb content in bulk KTa 1x Nb x O 3 (dotted curves in Fig. 4). Unexpectedly, the Curie temperature T C (x,r) nonmonotonically depends on Nb content x in assemblies of small (R = 15 nm) KTa 1x Nb x O 3 nanoparticles, when the fraction of spheres becomes less than 50% for the negative Vegard strain η (x) = 0.01x 0.03 (1 x) [Fig. 4(a)]. Such unexpected behavior could not be described as the consequence of particle shape changes, since the latter was constant under the increase of x. At the same time, the change of composition leads to the changes of the terms 4η(x)Q 12(x) 2η(x)(Q 11 (x)+2q 12 (x)) R0 2(x) s 11 (x)+2s 12 (x) R 2 s 11 (x)+s 12 (x) R 2 0 (x) R 2 and in Eqs. (4) and (5), proportional to the Vegard strain η (x), which changes in a strong way with composition x, according to Table III. Thus, the nonmonotonic behavior is a direct sequence of the rather strong increase of the Vegard strain with increasing x. When the fraction of spheres is higher than 50%, the Curie temperature monotonically and superlinearly increases with an x increase and can overcome the bulk Curie temperature by hundreds of degrees Kelvin for x>0.8. Figure 4(b) illustrates how the Curie temperature changes for the positive Vegard strain η (x) = 0.01x (1 x) and the same parameters as in Fig. 4(a). Qualitatively, the FIG. 4. (Color online) Curie temperature vs Nb content x in nanosized KTa 1x Nb x O 3. Plots are calculated for negative (a) and (c) and positive (b) and (d) Vegard strains. The particle radius is 15 nm in plots (a) and (b). The sphere fraction changes from 100% to 0%, with a step of 20% for different curves in the direction indicated by arrows. Plots (c) and (d) are calculated for different particle shapes (prolate ellipsoids and spheres as indicated by arrows) and radii 10, 20, and 40 nm (indicated by labels R i near the curves). Material parameters are listed in Tables II and III. FIG. 5. (Color online) Curie temperature vs particle radii R, calculated for Vegard strain at Nb content x = 0.3 (a), x = 0.5 (b), x = 0.9 (c), and x = 1 (d). The spheres fraction changes from 100% to 0%, with a step of 20% for different curves in the direction indicated by arrows. Material parameters are listed in Tables II and III
9 EFFECT OF VEGARD STRAINS ON THE EXTRINSIC... PHYSICAL REVIEW B 90, (2014) behavior for positive η (x) is complementary to the one for negative η (x) [compare Figs. 4(a) and 4(b)]. Namely, for η (x) > 0 sublinear x dependence of T C appears when the fraction of prolate ellipsoids becomes less than 50%. The Curie temperature monotonically and superlinearly increases with the Nb content increase and can overcome the bulk Curie temperature when the fraction of spheres is lower than 50%. These results support the statement that the principal behavior of the Curie temperature is governed by the Vegard strain sign (compression or tension), its absolute value, and particle shape (prolate or spherical one). In particular, one can see from Figs.4(a) and 4(b), which correspond to the opposite signs of the Vegard strain, that for positive η values, the curves for prolate ellipsoidal nanoparticles are located above the dotted curve corresponding to the bulk material; curves for spherical nanoparticles are located below the dotted curve. The curve sequence is the opposite for negative η values. The curve order and slope change with respect to the bulk dotted curve, with the changing fraction of spheres. In numbers, the transition temperature in the nanosized composite could be from tens to hundreds of degrees Kelvin lower or higher than in the bulk KTa 1x Nb x O 3. The smaller the particle radius R is, the stronger the deviation of the curves from the dotted bulk ones [Fig. 4(c)] is. Size effects are visible for the radii of less than 50 nm, and the minimal content of Nb required for the ferroelectricity appearance is different for bulk material (20%) and nanoparticles (from 10% to 30%), depending on the particle size, shape, and Vegard strain sign. In the case of the negative Vegard strain (η (x) < 0), the ellipsoids are characterized by the nonmonotonic dependence of the Curie temperature on the Nb content x, having a maximum at х = 0.6 and the second critical concentration of Nb, х = 0.95, at which ferroelectric order disappears. Figure 4(d) illustrates a model situation, when η (x) > 0 and other parameters are the same as for Fig. 4(c). One could see from this figure that it is possible to have a nonmonotonic dependence of the Curie temperature on Nb content for spherical nanoparticles of small radius; for the prolate ellipsoids, the Curie temperature monotonically increases with the increase of Nb content with the superlinear trend. Reconstructed dependences of the Curie temperature via particle radius are shown in Fig. 5 for different x and spheretoellipsoid ratios. At fixed content x, the Curie temperature T C tends to the bulk value with the particle radius increase. With the radius decrease, we see either the strong increase of T C proportional to R0 2/R2 for the negative product η (2Q 12 + Q 11 ) or ηq 12 for spherical or prolate nanoparticles, respectively [see Eq. (5)], or its rapid decrease up to T = 0 K at some critical radius R cr in the opposite case (compare top and bottom curves in Fig. 5). The critical radius R cr of the ferroelectricity disappearance exists for the positive product η (2Q 12 + Q 11 ) or ηq 12 for spherical or prolate nanoparticles, respectively. R cr increases with the increase of the η absolute value. The strong changes in the radius dependence of the Curie temperature T C appeared when the fraction of spheres varies from 100% to 0%. Actually, in the composite with compressed spherical nanoparticles (η <0), T C increases with the radius decrease. Increasing the fraction of prolate ellipsoids, T C gradually decreases, becomes lower than the bulk one, and rapidly decreases with the radius decrease in the composite with 50%, 20%, and 0% of spheres. Note, that the situation is vice versa for particles under tensile strains, η>0; here the temperature increases as the fraction of prolate particles increases. IV. SUMMARY We proposed a phenomenological description of size effects in ferroelectric nanoparticles taking into account Vegard strains caused by defect accumulation near the surface of the particle. Performing calculations and detailed quantitative comparison with experimental results on quasispherical KTa 1x Nb x O 3 nanoparticles (average radius 25 nm) allowed us to determine the key impact of the Vegard strain on the extrinsic size effects and reveal the essential (about 100 K) increase of the transition temperature in nanoparticles compared with bulk crystals. We also determined the dependence of the Vegard strains on the Nb content, and using this dependence, we reconstructed the content dependence of the solid solution Curie temperature. The dependence of the Curie temperature on the Nb content should be nonmonotonic for the small elongated KTa 1x Nb x O 3 nanoparticles (at size <30 nm). In this way, it is established that the key role in the origin of extrinsic size effects in nanoparticles belongs to the accumulation of intrinsic and extrinsic defects near the surface that cause local Vegard strains. The strains can govern the main features of the particles ferroelectric properties. [1] D. Yadlovker and S. Berger, Phys. Rev. B 71, (2005). [2] D. Yadlovker and S. Berger, Appl. Phys. Lett. 91, (2007). [3] D. Yadlovker and S. Berger, J. Appl. Phys.101, (2007). [4] M. H. Frey and D. A. Payne, Phys.Rev.B54, 3158 (1996). [5] Z. Zhao, V. Buscaglia, M. Viviani, M. T. Buscaglia, L. Mitoseriu, A. Testino, M. Nygren, M. Johnsson, and P. Nanni, Phys. Rev. B 70, (2004). [6] E. Erdem, H.C. Semmelhack, R. Bottcher, H. Rumpf, J. Banys, A. Matthes, H.J. Glasel, D. Hirsch, and E. Hartmann, J. Phys.: Condens. Matter. 18, 3861 (2006). [7] I. S. Golovina, S. P. Kolesnik, I. N. Geifman, and A. A. Andriiko, Ferroelectrics 416, 133 (2011). [8] I. S. Golovina, S. P. Kolesnik, V. Bryksa, V. V. Strelchuk, I. B. Yanchuk, I. N. Geifman, S. A. Khainakov, S. V. Svechnikov, and A. N. Morozovska, Physica B 407, 614 (2012). [9] I. S. Golovina, B. D. Shanina, S. P. Kolesnik, I. N. Geifman, and A. A. Andriiko, Phys. Status Solidi B 249, 2263 (2012). [10] I. S. Golovina, I. N. Geifman, and М. Prokopiv, Ukr. Phys. J. 57, 63 (2012). [11] I. S. Golovina, V. P. Bryksa, V. V. Strelchuk, I. N. Geifman, and A. A. Andriiko, J. Appl. Phys. 113, (2013)
10 ANNA N. MOROZOVSKA et al. PHYSICAL REVIEW B 90, (2014) [12] I. S. Golovina, V. P. Bryksa, V. V. Strelchuk, and I. N. Geifman, Functional Materials 20, 75 (2013). [13] I. S. Golovina, B. D. Shanina, S. P. Kolesnik, I. N. Geifman, and A. A. Andriiko, J. Appl. Phys. 114, (2013). [14] P. Perriat, J. C. Niepce, and G. Caboche, J. Therm. Anal. Calorim. 41, 635 (1994). [15] H. Huang, C. Q Sun, and P. Hing, J. Phys.: Condens. Matter 12, L127 (2000). [16] H. Haitao, C. Q. Sun, Z. Tianshu, and P. Hing, Phys.Rev.B63, (2001). [17] A. N. Morozovska, E. A. Eliseev, and M. D. Glinchuk, Phys. Rev. B 73, (2006). [18] A. N. Morozovska, M. D. Glinchuk, and E. A. Eliseev, Phys. Rev. B 76, (2007). [19] M. D. Glinchuk, E. A. Eliseev, A. N. Morozovska, and R. Blinc, Phys. Rev. B 77, (2008). [20] A. N. Morozovska, M. D. Glinchuk, Rakesh K. Behera, B. Y. Zaylichniy, Chaitanya S. Deo, and E. A. Eliseev, Phys. Rev. B 84, (2011). [21] E. A. Eliseev, M. D. Glinchuk, V. V. Khist, C.W. Lee, C. S. Deo, R. K. Behera, and A. N. Morozovska, J. Appl. Phys. 113, (2013). [22] W. Ma. Appl. Phys. A 96, 915 (2009). [23] V. A. Shchukin and D. Bimberg, Rev. Mod. Phys., 71, 1125 (1999). [24] A. K. Tagantsev, G. Gerra, and N. Setter, Phys. Rev. B 77, (2008). [25] R. Kretschmer and K. Binder, Phys.Rev.B20, 1065 (1979). [26] C.L. Jia, V. Nagarajan, J.Q. He, L. Houben, T. Zhao, R. Ramesh, K. Urban, and R. Waser, Nat. Mater (2007). [27] E. A. Eliseev, A. N. Morozovska, M. D. Glinchuk, and R. Blinc, Phys. Rev. B 79, (2009). [28] A. K. Tagantsev and G. Gerra, J. Appl. Phys. 100, (2006). [29] F. Wang, Z. Pang, L. Lin, S. Fang, Y. Dai, and S. Han, Phys. Rev. B 80, (2009). [30] J. Carrasco, F. Illas, N. Lopez, E. A. Kotomin, Yu. F. Zhukovskii, R. A. Evarestov, Yu. A. Mastrikov, S. Piskunov, and J. Maier, Phys. Rev. B 73, (2006). [31] H. Jin, Y. Dai, BaiBiao Huang, and M.H. Whangbo, Appl. Phys. Lett. 94, (2009). [32] K. R. Brown, and D. A. Bonnell, J. Am. Ceram. Soc. 82, 2431 (1999). [33] Y. Xiao, V. B. Shenoy, and K. Bhattacharya, Phys. Rev. Lett. 95, (2005). [34] B. W. Sheldon and V. B. Shenoy, Phys.Rev.Lett.106, (2011). [35] G. B. Stephenson and M. J. Highland, Phys.Rev.B84, (2011). [36] G. Catalan and James F. Scott, Adv. Mater. 21, 2463 (2009). [37] X. Zhang, A. M. Sastry, and W. Shyy, J. Electrochem. Soc. 155, A542 (2008). [38] D. A. Freedman, D. Roundy, and T. A. Arias, Phys.Rev.B80, (2009). [39] T. Ohnishi, K. Shibuya, T. Yamamoto, and M. Lippmaa, J. Appl. Phys. 103, (2008). [40] C. M. Brooks, L. F. Kourkoutis, T. Heeg, J. Schubert, D. A. Muller, and D. G. Schlom, Appl. Phys. Lett. 94, (2009). [41] P. S. Sankara, R. Krishnan, A. N. Morozovska, E. A. Eliseev, Q. M. Ramasse, D.Kepaptsoglou, W.I. Liang, Y.H. Chu, P. Munroe, and V. Nagarajan, J.Appl. Phys.115, (2014). [42] A. N. Morozovska, E. A. Eliseev, P. S. Sankara Rama Krishnan, A. Tselev, E. Strelkov, A. Borisevich, O. V. Varenyk, N. V. Morozovsky, P. Munroe, S. V. Kalinin, and V. Nagarajan, Phys. Rev. B 89, (2014). [43] M. S. Kilic, M. Z. Bazant, and A. Ajdari, Phys.Rev.E75, (2007). [44] M. S. Kilic, M. Z. Bazant, and A. Ajdari, Phys.Rev.E75, (2007). [45] M. E. Lines and A. M. Glass, Principles and Application of Ferroelectrics and Related Materials (Clarendon Press, Oxford, 1977). [46] S. Triebwasser, Phys. Rev. 114, 63 (1959). [47] L. D. Landau and E. M. Lifshitz, Electrodynamics of Continuous Media (Butterworth Heinemann, Oxford, 1980). [48] J. Wang, A. K. Tagantsev, and N. Setter, Phys.Rev.B83, (2011). [49] J. H. Barrett, Phys. Rev. 86, 118 (1952). [50] H. Uwe and T. Sakudo, J. Phys. Soc. Jpn. 38, 183 (1975). [51] L. Liang, Y. L. Li, L.Q. Chen, S. Y. Hu, and G.H. Lu, J. Appl. Phys. 106, (2009)
APPENDIX A Landau FreeEnergy Coefficients
APPENDIX A Landau FreeEnergy Coefficients LongQing Chen Department of Materials Science and Engineering, The Pennsylvania State University, University Park, Pennsylvania 180 USA The thermodynamics of
More informationElectric field dependent sound velocity change in Ba 1 x Ca x TiO 3 ferroelectric perovskites
Indian Journal of Pure & Applied Physics Vol. 49, February 2011, pp. 132136 Electric field dependent sound velocity change in Ba 1 x Ca x TiO 3 ferroelectric perovskites Dushyant Pradeep, U C Naithani
More informationThe anomalies of the properties of nanomaterials related to the distribution of the grain sizes
The anomalies of the properties of nanomaterials related to the distribution of the grain sizes M.D.Glinchuk, P.I.Bykov Institute for Problems of Materials Science, NASc of Ukraine, Kjijanovskogo 3, 368
More informationSurface stress and relaxation in metals
J. Phys.: Condens. Matter 12 (2000) 5541 5550. Printed in the UK PII: S09538984(00)113864 Surface stress and relaxation in metals P M Marcus, Xianghong Qian and Wolfgang Hübner IBM Research Center, Yorktown
More informationInterfacial Coherency and Ferroelectricity of BaTiO 3 /SrTiO 3 Superlattice Films
Boise State University ScholarWorks Physics Faculty Publications and Presentations Department of Physics 12182007 Interfacial Coherency and Ferroelectricity of BaTiO 3 /SrTiO 3 Superlattice Films Y.
More informationLattice Expansion of (Ga,Mn)As: The Role of Substitutional Mn and of the Compensating Defects
Vol. 108 (2005) ACTA PHYSICA POLONICA A No. 5 Proceedings of the XXXIV International School of Semiconducting Compounds, Jaszowiec 2005 Lattice Expansion of (Ga,Mn)As: The Role of Substitutional Mn and
More informationMaterial parameters for electrostriction
Material parameters for electrostriction Yuri M. Shkel and Daniel J. Klingenberg a) Department of Chemical Engineering and Rheology Research Center, University of Wisconsin, Madison, Wisconsin 53706 Received
More informationPhase Transitions in Strontium Titanate
Phase Transitions in Strontium Titanate Xinyue Fang Department of Physics, University of Illinois at UrbanaChampaign Abstract Strontium Titanate SrTiO 3 (STO) is known to undergo an antiferrodistortive
More information(a) (b) Supplementary Figure 1. (a) (b) (a) Supplementary Figure 2. (a) (b) (c) (d) (e)
(a) (b) Supplementary Figure 1. (a) An AFM image of the device after the formation of the contact electrodes and the top gate dielectric Al 2 O 3. (b) A line scan performed along the white dashed line
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationStructure and Dynamics : An Atomic View of Materials
Structure and Dynamics : An Atomic View of Materials MARTIN T. DOVE Department ofearth Sciences University of Cambridge OXFORD UNIVERSITY PRESS Contents 1 Introduction 1 1.1 Observations 1 1.1.1 Microscopic
More informationColloidal Particles at Liquid Interfaces: An Introduction
1 Colloidal Particles at Liquid Interfaces: An Introduction Bernard P. Binks and Tommy S. Horozov Surfactant and Colloid Group, Department of Chemistry, University of Hull, Hull, HU6 7RX, UK 1.1 Some Basic
More informationElectrical Properties
Electrical Properties Electrical Conduction R Ohm s law V = IR I l Area, A V where I is current (Ampere), V is voltage (Volts) and R is the resistance (Ohms or ) of the conductor Resistivity Resistivity,
More informationPhase Transitions in Relaxor Ferroelectrics
Phase Transitions in Relaxor Ferroelectrics Matthew Delgado December 13, 2005 Abstract This paper covers the properties of relaxor ferroelectrics and considers the transition from the paraelectric state
More informationClassification of Dielectrics & Applications
Classification of Dielectrics & Applications DIELECTRICS NonCentro Symmetric Piezoelectric Centro Symmetric Pyroelectric Non Pyroelectric Ferroelectrics NonFerroelectric Piezoelectric Effect When
More informationFerroelectric materials contain one or more polar axes along which a spontaneous
Chapter 3 Ferroelectrics 3.1 Definition and properties Ferroelectric materials contain one or more polar axes along which a spontaneous polarization can be developed below the material s Curie temperature.
More informationCalculation and Analysis of the Dielectric Functions for BaTiO 3, PbTiO 3, and PbZrO 3
CHINESE JOURNAL OF PHYSICS VOL. 1, NO. 3 June 213 Calculation and Analysis of the Dielectric Functions for BaTiO 3, PbTiO 3, and PbZrO 3 Chao Zhang and Dashu Yu School of Physics & Electronic Information
More informationAberrationcorrected TEM studies on interface of multilayeredperovskite systems
Aberrationcorrected TEM studies on interface of multilayeredperovskite systems By Lina Gunawan (0326114) Supervisor: Dr. Gianluigi Botton November 1, 2006 MSE 702(1) Presentation Outline Literature Review
More informationReentrant phase in nanoferroics induced by the flexoelectric and Vegard effects
Reentrant phase in nanoferroics induced y the flexoelectric and Vegard effects Anna N. Morozovska 1 and Maya D. Glinchuk, 1 Institute of Physics, National Academy of Sciences of Ukraine, 46, pr. Nauky,
More informationStructure and Curie temperature of Y 2 Fe 17 x Cr x
Vol. 46 No. 4 SCIENCE IN CHINA (Series G) August 2003 Structure and Curie temperature of Y 2 Fe 17 x Cr x HAO Shiqiang ( ) 1 & CHEN Nanxian ( ) 1,2 1. Department of Physics, Tsinghua University, Beijing
More informationInterfacial effects in electromagnetic coupling within piezoelectric phononic crystals
Acta Mech Sin (29) 25:95 99 DOI 1.17/s149821y RESEARCH PAPER Interfacial effects in electromagnetic coupling within pieoelectric phononic crystals F. J. Sabina A. B. Movchan Received: 14 July 28 / Accepted:
More informationAdaptive ferroelectric states in systems with low domain wall energy: Tetragonal microdomains
Adaptive ferroelectric states in systems with low domain wall energy: Tetragonal microdomains Y. M. Jin, Y. U. Wang, A. G. Khachaturyan, J. F. Li, and D. Viehland Citation: Journal of Applied Physics 94,
More informationI. B. Misirlioglu*, M. Yildiz. Faculty of Engineering and Natural Sciences, Sabanci University, Tuzla/Orhanli, Istanbul, Turkey.
Interdigitated Finger Electrode and Sandwich Type Ferroelectric Nano Film Capacitors: A Comparison of the Effect of Electrostatic Boundary Conditions and Defects I. B. Misirlioglu*, M. Yildiz Faculty of
More informationImpact of size and temperature on thermal expansion of nanomaterials
PRAMANA c Indian Academy of Sciences Vol. 84, No. 4 journal of April 205 physics pp. 609 69 Impact of size and temperature on thermal expansion of nanomaterials MADAN SINGH, and MAHIPAL SINGH 2 Department
More informationMustafa Uludogan 1, Tahir Cagin, William A. Goddard, III Materials and Process Simulation Center, Caltech, Pasadena, CA 91125, U.S.A.
Ab Initio Studies On Phase Behavior of Barium Titanate Mustafa Uludogan 1, Tahir Cagin, William A. Goddard, III Materials and Process Simulation Center, Caltech, Pasadena, CA 91125, U.S.A. 1 Physics Department,
More informationEffects of Particle Shape and Microstructure on Effective Nonlinear Response
Commun. Theor. Phys. (Beijing, China) 36 (2001) pp. 365 369 c International Academic Publishers Vol. 36, No. 3, September 15, 2001 Effects of Particle Shape and Microstructure on Effective Nonlinear Response
More informationSURFACE ACOUSTIC WAVE FERROELECTRIC PHONONIC CRYSTAL TUNABLE BY ELECTRIC FIELD
NANOSYSTEMS: PHYSICS, CHEMISTRY, MATHEMATICS, 2013, 4 (5), P. 630 634 SURFACE ACOUSTIC WAVE FERROELECTRIC PHONONIC CRYSTAL TUNABLE BY ELECTRIC FIELD V. P. Pashchenko 1,2 1 Saint Petersburg State Polytechnical
More informationA METHOD FOR CALCULATING SURFACE STRESS AND ELASTIC CONSTANTS BY MOLECULAR DYNAMICS
A METHOD FOR CALCULATING SURFACE STRESS AND ELASTIC CONSTANTS BY MOLECULAR DYNAMICS Satoshi Izumi Dept. of Mechanical Engineering, Univ. of Tokyo., JAPAN Shotaro Hara Dept. of Mechanical Engineering, Univ.
More informationPLEASE SCROLL DOWN FOR ARTICLE
This article was downloaded by: [Uniwersytet Slaski] On: 14 October 2008 Access details: Access Details: [subscription number 903467288] Publisher Taylor & Francis Informa Ltd Registered in England and
More informationPublication I. c 2010 American Physical Society. Reprinted with permission.
Publication I Tyunina, M., Narkilahti, J., Plekh, M., Oja, R., Nieminen, R.M., Dejneka, A., and Trepakov, V. Evidence for StrainInduced Ferroelectric Order in Epitaxial ThinFilm KTaO 3. Physical Review
More informationRoomtemperature tunable microwave properties of strained SrTiO 3 films
JOURNAL OF APPLIED PHYSICS VOLUME 96, NUMBER 11 1 DECEMBER 2004 Roomtemperature tunable microwave properties of ed SrTiO 3 films Wontae Chang, a) Steven W. Kirchoefer, Jeffrey M. Pond, Jeffrey A. Bellotti,
More informationChapter 3 Properties of Nanostructures
Chapter 3 Properties of Nanostructures In Chapter 2, the reduction of the extent of a solid in one or more dimensions was shown to lead to a dramatic alteration of the overall behavior of the solids. Generally,
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationNoise Shielding Using Acoustic Metamaterials
Commun. Theor. Phys. (Beijing, China) 53 (2010) pp. 560 564 c Chinese Physical Society and IOP Publishing Ltd Vol. 53, No. 3, March 15, 2010 Noise Shielding Using Acoustic Metamaterials LIU Bin ( Ê) and
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More informationConstructing LandauGinzburgDevonshire Type Models for Ferroelectric Systems Based on Symmetry
701 GFER A 3395 October 18, 008 11:19 GFER #3395, VOL 375, ISS 1 Constructing LandauGinzburgDevonshire Type Models for Ferroelectric Systems Based on Symmetry WENWU CAO QUERY SHEET This page lists questions
More informationPhenomenological Theory of a Single Domain Wall in Uniaxial Trigonal Ferroelectrics: Lithium Niobate and Lithium Tantalate
Accepted in PRB, 005 Phenomenological Theory of a Single Domain Wall in Uniaxial Trigonal Ferroelectrics: Lithium Niobate and Lithium Tantalate David A Scrymgeour and Venkatraman Gopalan Department of
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More informationof Nebraska  Lincoln
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Xiao Cheng Zeng Publications Published Research  Department of Chemistry 1012006 Homogeneous nucleation at high supersaturation
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationElectrical material properties
Electrical material properties U = I R Ohm s law R = ρ (l/a) ρ resistivity l length σ = 1/ρ σ conductivity A area σ = n q μ n conc. of charge carriers q their charge μ their mobility μ depends on T, defects,
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationarxiv:condmat/ v1 [condmat.disnn] 25 Apr 2000
Griffiths phase manifestation in disordered dielectrics V.A.Stephanovich Institute of Mathematics, University of Opole, Oleska 8, 55, Opole, Poland and Institute of Semiconductor Physics NAS of Ukraine,
More informationFlexible PiezoelectricInduced Pressure Sensors for Static. Measurements Based on Nanowires/Graphene Heterostructures
Flexible PiezoelectricInduced Pressure Sensors for Static Measurements Based on Nanowires/Graphene Heterostructures Zefeng Chen,, Zhao Wang,, Xinming Li,*, Yuxuan Lin, Ningqi Luo, Mingzhu Long, Ni Zhao,
More informationNonlinear resistance of twodimensional electrons in crossed electric and magnetic fields
Nonlinear resistance of twodimensional electrons in crossed electric and magnetic fields Jing Qiao Zhang and Sergey Vitkalov* Department of Physics, City College of the City University of New York, New
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationDomain Structures in Epitaxial Ferroelectric Thin Films
Domain Structures in Epitaxial Ferroelectric Thin Films By: Brian Smith S1711377 Supervised by: Prof. dr. Beatrix Noheda February 2009 1 TABLE OF CONTENTS Introduction. 3 1. Background 4 2. Experimental..
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More informationChapter 10: Steady Heat Conduction
Chapter 0: Steady Heat Conduction In thermodynamics, we considered the amount of heat transfer as a system undergoes a process from one equilibrium state to another hermodynamics gives no indication of
More informationSolutions for the electric potential and field distribution in cylindrical coreshell nanoparticles using the image charge method
Solutions for the electric potential and field distribution in cylindrical coreshell nanoparticles using the image charge method Nader Daneshfar, and Nasrin Moradbeigi Citation: AIP Advances 5, 1714 (15);
More informationPiezo materials. Actuators Sensors Generators Transducers. Piezoelectric materials may be used to produce e.g.: Piezo materials Ver1404
Noliac Group develops and manufactures piezoelectric materials based on modified lead zirconate titanate (PZT) of high quality and tailored for custom specifications. Piezoelectric materials may be used
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationAddition 1. Shear Stack Piezoelectric Elements and Shear Effect Basics
120 Addition 1 Shear Stack Piezoelectric Elements and Shear Effect Basics Introduction The STM scanner built up in this work is a Besocke type scanner (see room temperature STM instrumental chapter). The
More informationSynthesis and Ferroelectric Properties of KNO 3 films
Synthesis and Ferroelectric Properties of KNO 3 films Shahid Ramay and Muhammad Sabieh Anwar LUMS School of Science and Engineering Friday, August, 20, 2010 Potassium nitrate (KNO 3 ) shows ferroelectric
More informationElectricity & Magnetism Study Questions for the Spring 2018 Department Exam December 4, 2017
Electricity & Magnetism Study Questions for the Spring 2018 Department Exam December 4, 2017 1. a. Find the capacitance of a spherical capacitor with inner radius l i and outer radius l 0 filled with dielectric
More informationA General Equation for Fitting Contact Area and Friction vs Load Measurements
Journal of Colloid and Interface Science 211, 395 400 (1999) Article ID jcis.1998.6027, available online at http://www.idealibrary.com on A General Equation for Fitting Contact Area and Friction vs Load
More informationA chemomechanical model coupled with thermal effect on the hollow core shell electrodes in lithiumion batteries
Accepted Manuscript A chemomechanical model coupled with thermal effect on the hollow core shell electrodes in lithiumion batteries Bin Hu, Zengsheng Ma, Weixin Lei, Youlan Zou, Chunsheng Lu PII: S20950349(17)30096X
More informationOrientation dependence of electromechanical properties of relaxor based ferroelectric single crystals
J Mater Sci (2011) 46:63 68 DOI 10.1007/s108530104804x Orientation dependence of electromechanical properties of relaxor based ferroelectric single crystals Yang Xiang Rui Zhang Wenwu Cao Received:
More informationSCIENCE CHINA Physics, Mechanics & Astronomy. Electronic structure and optical properties of NZn codoped Ga 2 O 3
SCIENCE CHINA Physics, Mechanics & Astronomy Article April 2012 Vol.55 No.4: 654 659 doi: 10.1007/s1143301246869 Electronic structure and optical properties of NZn codoped Ga 2 O 3 YAN JinLiang *
More informationA Simulation Model of Fluid Flow and Streamlines Induced by NonUniform Electric Field
Proceedings of the 4th International Middle East Power Systems Conference (MEPCON ), Cairo University, Egypt, December 9,, Paper ID 8. A Simulation Model of Fluid Flow and Streamlines Induced by NonUniform
More informationPHY 481/581. Some classical/quantum physics for the nanometer length scale.
PHY 481/581 Some classical/quantum physics for the nanometer length scale http://creativecommons.org/licenses/byncsa/3.0/ 1 What is nanoscience? the science of materials whose properties scale with
More informationAP Physics C. Electric Potential and Capacitance. Free Response Problems
AP Physics C Electric Potential and Capacitance Free Response Problems 1. Two stationary point charges + are located on the yaxis at a distance L from the origin, as shown above. A third charge +q is
More informationThe nature of special points on unit cell parameters temperature dependences for crystal substances
Z. Kristallogr. Suppl. 26 (2007) 447452 by Oldenbourg Wissenschaftsverlag, München 447 The nature of special points on unit cell parameters temperature dependences for crystal substances Stanislav K.
More informationCONTRASTING BEHAVIOR OF FREESTANDING AND EMBEDDED MAGNETIC NANOPARTICLES
(c) Romanian RRP 65(No. Reports in 3) Physics, 832 840 Vol. 2013 65, No. 3, P. 832 840, 2013 Dedicated to Professor Valentin I. Vlad s 70 th Anniversary CONTRASTING BEHAVIOR OF FREESTANDING AND EMBEDDED
More informationGraded Ferroelectric Capacitors with Robust Temperature Characteristics. Abstract
Preprint Graded Ferroelectric Capacitors with Robust Temperature Characteristics Mohamed Y. ElNaggar, Kaushik Dayal, David G. Goodwin, and Kaushik Bhattacharya Division of Engineering & Applied Science
More informationMultiple Image Method for the Two Conductor Spheres in a Uniform Electrostatic Field
Commun. Theor. Phys. 57 (2012) 1066 1070 Vol. 57, No. 6, June 15, 2012 Multiple Image Method for the Two Conductor Spheres in a Uniform Electrostatic Field GAO Xin (Ô ), 1,2 HU Lin ( ), 1, and SUN Gang
More informationFerroelectrics and ferroelectric domains
Ferroelectrics and ferroelectric domains MatjažPanjan mentor: dr. Peter Prelovšek. April 003 Abstract This seminar gives introduction to ferroelectricity, ferroelectric domains and domain walls. There
More informationThe Effect of Dipole Boron Centers on the Electroluminescence of Nanoscale Silicon p + n Junctions
The Effect of Dipole Boron Centers on the Electroluminescence of Nanoscale Silicon p + n Junctions Nikolay Bagraev a, Leonid Klyachkin a, Roman Kuzmin a, Anna Malyarenko a and Vladimir Mashkov b a Ioffe
More informationElectric fields in matter
Electric fields in matter November 2, 25 Suppose we apply a constant electric field to a block of material. Then the charges that make up the matter are no longer in equilibrium: the electrons tend to
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationV. Electrostatics Lecture 24: Diffuse Charge in Electrolytes
V. Electrostatics Lecture 24: Diffuse Charge in Electrolytes MIT Student 1. PoissonNernstPlanck Equations The NernstPlanck Equation is a conservation of mass equation that describes the influence of
More informationTransport properties through doublemagneticbarrier structures in graphene
Chin. Phys. B Vol. 20, No. 7 (20) 077305 Transport properties through doublemagneticbarrier structures in graphene Wang SuXin( ) a)b), Li ZhiWen( ) a)b), Liu JianJun( ) c), and Li YuXian( ) c) a)
More informationSupplementary Figure 1 Extracting process of wetting ridge profiles. a14, An extraction example of a ridge profile for E 16 kpa.
Supplementary Figure 1 Extracting process of wetting ridge profiles. a14, An extraction example of a ridge profile for E 16 kpa. An original image (a1) was binarized, as shown in a2, by Canny edge detector
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationDomain switching and electromechanical properties of pulse poled Pb Zn 1Õ3 Nb 2Õ3 O 3 PbTiO 3 crystals
JOURNAL OF APPLIED PHYSICS VOLUME 89, NUMBER 1 1 JANUARY 2001 Domain switching and electromechanical properties of pulse poled Pb Zn 1Õ3 Nb 2Õ3 O 3 PbTiO 3 crystals Hanxing Yu, Venkat Gopalan, Jürgen Sindel,
More informationLecture 7. Properties of Materials
MIT 3.00 Fall 2002 c W.C Carter 55 Lecture 7 Properties of Materials Last Time Types of Systems and Types of Processes Division of Total Energy into Kinetic, Potential, and Internal Types of Work: Polarization
More informationarxiv:condmat/ v1 [condmat.other] 5 Jun 2004
arxiv:condmat/0406141v1 [condmat.other] 5 Jun 2004 Moving Beyond a Simple Model of Luminescence Rings in Quantum Well Structures D. Snoke 1, S. Denev 1, Y. Liu 1, S. Simon 2, R. Rapaport 2, G. Chen 2,
More informationGiant Flexoelectric Effect in Ferroelectric Epitaxial Thin Films
Giant Flexoelectric Effect in Ferroelectric Epitaxial Thin Films Daesu Lee, 1 A. Yoon, 2 S. Y. Jang, 1 J.G. Yoon, 3 J.S. Chung, 4 M. Kim, 2 J. F. Scott, 5 and T. W. Noh 1,* 1 ReCFI, Department of Physics
More informationEXISTENCE AND UNIQUENESS FOR A THREE DIMENSIONAL MODEL OF FERROMAGNETISM
1 EXISTENCE AND UNIQUENESS FOR A THREE DIMENSIONAL MODEL OF FERROMAGNETISM V. BERTI and M. FABRIZIO Dipartimento di Matematica, Università degli Studi di Bologna, P.zza di Porta S. Donato 5, I4126, Bologna,
More informationBoundary Conditions in Fluid Mechanics
Boundary Conditions in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University The governing equations for the velocity and pressure fields are partial
More informationA test of the method of images at the surface of molecular materials
JOURNAL OF CHEMICAL PHYSICS VOLUME 120, NUMBER 8 22 FEBRUARY 2004 A test of the method of images at the surface of molecular materials A. Eilmes Faculty of Chemistry, Jagiellonian University, Ingardena
More informationModified MaxwellGarnett equation for the effective transport coefficients in inhomogeneous media
J. Phys. A: Math. Gen. 3 (998) 7227 7234. Printed in the UK PII: S03054470(98)939762 Modified MaxwellGarnett equation for the effective transport coefficients in inhomogeneous media Juris Robert Kalnin
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationFerroelectric Materials
Ferroelectric Materials The permanent electric dipole moment possessed by all pyroelectric [polar] materials may, in certain cases, be reoriented by the application of an electric field. Such crystals
More informationSeminars in Nanosystems  I
Seminars in Nanosystems  I Winter Semester 2011/2012 Dr. Emanuela Margapoti Emanuela.Margapoti@wsi.tum.de Dr. Gregor Koblmüller Gregor.Koblmueller@wsi.tum.de Seminar Room at ZNN 1 floor Topics of the
More informationEquivalence of total force (and torque) for two formulations of the Lorentz law
Equivalence of total force (and torque) for two formulations of the Lorentz law Masud Mansuripur, Armis R. Zakharian, and Jerome V. Moloney College of Optical Sciences, The University of Arizona, Tucson,
More informationQuantum dot heterostructures: fabrication, properties, lasers Review
SEMICONDUCTORS VOLUME 32, NUMBER 4 APRIL 1998 Quantum dot heterostructures: fabrication, properties, lasers Review N. N. Ledentsov, V. M. Ustinov, V. A. Shchukin. P. S. Kop ev, and Zh. I. Alferov A. F.
More informationF 10 Electrical Poling of Polymers
University of Potsdam, Institute of Physics Advanced lab experiments May 28, 2002 F 10 Electrical Poling of Polymers Tutor: Dr. Michael Wegener * Contents 1 Introduction 2 2 Tasks 3 3 Theoretical background
More information5 Topological defects and textures in ordered media
5 Topological defects and textures in ordered media In this chapter we consider how to classify topological defects and textures in ordered media. We give here only a very short account of the method following
More informationPIC/MCC Simulation of Radio Frequency Hollow Cathode Discharge in Nitrogen
PIC/MCC Simulation of Radio Frequency Hollow Cathode Discharge in Nitrogen HAN Qing ( ), WANG Jing ( ), ZHANG Lianzhu ( ) College of Physics Science and Information Engineering, Hebei Normal University,
More informationSpins and spinorbit coupling in semiconductors, metals, and nanostructures
B. Halperin Spin lecture 1 Spins and spinorbit coupling in semiconductors, metals, and nanostructures Behavior of nonequilibrium spin populations. Spin relaxation and spin transport. How does one produce
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More information2.1 Experimental and theoretical studies
Chapter 2 NiO As stated before, the firstrow transitionmetal oxides are among the most interesting series of materials, exhibiting wide variations in physical properties related to electronic structure.
More informationComplete band gaps in twodimensional phononic crystal slabs
Complete band gaps in twodimensional phononic crystal slabs A. Khelif, 1 B. Aoubiza, 2 S. Mohammadi, 3 A. Adibi, 3 and V. Laude 1 1 Institut FEMTOST, CNRS UMR 6174, Université de FrancheComté, Besançon,
More informationProperties of Individual Nanoparticles
TIGP Introduction technology (I) October 15, 2007 Properties of Individual Nanoparticles Clusters 1. Very small  difficult to image individual nanoparticles. 2. New physical and/or chemical properties
More informationClass XI Physics. Ch. 9: Mechanical Properties of solids. NCERT Solutions
Downloaded from Class XI Physics Ch. 9: Mechanical Properties of solids NCERT Solutions Page 242 Question 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More information